Manufacture of Different Types
Lavinia Ardelean, Cristina Bortun, Angela Podariu and Laura Rusu
“Victor Babes” University of Medicine and Pharmacy Timisoara
The development of resins represented a great step forward in dental technique, the first
thermopolymerisable acrylic resins being developed in 1936. Acrylic resins are better known
as poly(methyl methacrylate) or PMMA. They are synthetically obtained materials that can
be modelled, packed or injected into molds during an initial plastic phase which solidify
through a chemical reaction-polymerisation (Phoenix et al., 2004). However, the
disadvantages of thermopolymerisable acrylic resins, connected to increased porosity, high
water retention, volume variations and irritating effect of the residual monomer (organic
solvent, hepatotoxic), awkward wrapping system, difficult processing, together with the
polymer development, have led to alternative materials such as polyamides (nylon), acetal
resins, epoxy resins, polystyrene, polycarbonate resins etc. (Negrutiu et al., 2001).
Thermoplastic resins have been used in dental medicine for fifty years. In the meantime, their
use has spread due to their superior characteristics. Their ongoing development has yielded
new classes of more and more advanced materials and technologies, which make possible the
manufacturing of dentures with better splinting properties then traditional dentures.
2. Thermoplastic resins used in dentistry
The classification of resins according to DIN EN ISO–1567 comprises:
From the point of view of their composition, as far as thermoplastic resins are concerned, we
can distinguish among: acetal resins, polycarbonate resins (belonging to the group of
polyester resins), acrylic resins, polyamides (nylons).
Usage of thermoplastic resins in dental medicine has significantly grown in the last decade.
The technology is based on plasticising the material using only thermal processing in the
absence of any chemical reaction. The possibility of injecting the plasticized resin into a
mold has opened a new perspective to full denture and removable partial denture
Successive alterations to the chemical composition led to the diversification of their range of
application, so that at present thermoplastic materials are suitable for the manufacturing of
removable partial dentures which totally or partially eliminate the metallic component,
resulting in the so-called “metal-free removable partial dentures” (Bortun et al., 2006).
Thermoplastic – Composite Materials
Type Class (manufacturing) Group (presentation form)
Type 1 thermopolymerisable resins (> 65°C) Groupe 1: bicomponent - powder and liquid
Groupe 2: monocomponent
Type 2 autopolymerisable resins (< 65°C) Groupe 1: bicomponent - powder and liquid
Groupe 2: bicomponent - powder and
Type 3 thermoplastic resins Monocomponent system: grains in
Type 4 photopolymerisable resins Monocomponent system
Type 5 microwave polymerisable resins Bicomponent system
Table 1. The classification of resins according to DIN EN ISO–1567
Indications for thermoplastic resins include: partial dentures, preformed clasps, partial
denture frameworks, temporary or provisional crowns and bridges, full dentures,
orthodontic appliances, myofunctional therapy devices, anti-snoring devices, different types
of mouthguards and splints.
2.1 Thermoplastic acetal
Thermoplastic acetal is a poly(oxy-methylene)-based material, which as a homopolymer has
good short-term mechanical properties, but as a copolymer has better long-term stability
(Arikan et al., 2005).
Acetal resin is very strong, resists wear and fracturing, and it’s flexible, which makes it an ideal
material for pre-formed clasps for partial dentures, single pressed unilateral partial dentures,
partial denture frameworks, provisional bridges, occlusal splints and implant abutments,
partial denture frameworks, artificial teeth for removable dentures, orthodontic appliances.
Acetal resins resist occlusal wear and are well suited for maintaining vertical dimension
during provisional restorative therapy. Acetal does not have the natural translucency and
esthetic appearance of thermoplastic acrylic and polycarbonate (Ozkan et al., 2005).
2.2 Thermoplastic polyamide (nylon)
Thermoplastic nylon is a polyamidic resin derived from diamine and dibasic acid
monomers. Nylon is a versatile material, suitable for a broad range of applications.
Nylon exhibits high flexibility, physical strength, heat and chemical resistance. It can be
easily modified to increase stiffness and wear resistance. Because of its excellent balance of
strength, ductility and heat resistance, nylon is an outstanding candidate for metal
They are used primarily for tissue supported removable dentures because their stiffness makes
them unsuitable for usage as occlusal rests or denture parts that need to be rigid. Because of its
flexibility, it can’t maintain vertical dimension when used in direct occlusal forces.
Nylon is a little more difficult to adjust and polish, but the resin can be semi-translucent and
provides excellent esthetics (Donovan & Cho, 2003).
Manufacture of Different Types of Thermoplastic
Resin type Main
Resistance Durity Flexibility Esthetics Biocompati-
very good very
medium good very good
diamin good high medium or very
on the material
very good very good
Table 2. Comparative aspects of acetalic and polyamidic thermoplastic resins
2.3 Thermoplastic polyester
Another group of thermoplastic materials used in dentistry are polyester resins. These resins
melt between 230-290ºC and the technology implies casting into molds.
Polycarbonate resins are particular polyester materials. They exhibit fracture strength and
flexibility, but the wear resistance is lower when compared to acetal resins. However,
polycarbonates have a natural translucency and finishes very well, which make them proper
for producing temporary restorations. They are not suitable for partial denture frameworks
(Negrutiu et al., 2005).
At present, there are several manufacturers that provide thermoplastic materials for dental
use: The Flexite Company, Valplast Int. Corp., Girrbach Dental, Bredent, Dentsply, DR
Dental Resource Inc., If Dental-Pressing Dental etc.
Fig. 1. (a), (c) Cartridges of different thermoplastic resins, (b) The granular aspect of the
Thermoplastic – Composite Materials
2.4 Presentation form and injection
Thermoplastic materials can be polymerised or prepolymerised and they can be found in
granular form, with low molecular weight, already wrapped in cartridges which eliminates
dosage errors - Fig. 1.
They have a low plasticizing temperature and exhibit a high rigidity in spite of their low
molecular weight. Their plasticizing temperature is 200-250°C.
After thermal plasticization in special devices, the material is injected under pressure into a
mold, without any chemical reactions. The metallic cartridges containing thermoplastic
grains are heated to plasticize the resin. The cartridges are set in place into the injecting unit
and pressure of 6-8 barrs is used to force the plasticized resin to fill the mold. Pressure,
temperature and injecting time are automatically controlled by the injecting unit. This
results in compact dentures with excellent esthetics and good compatibility.
Injecting thermoplastic resins into molds is not a common technology in dental laboratories
because the need of expensive equipment and this could be a disadvantage.
We will describe the manufacturing process of metal-free removable partial dentures made
off several thermoplastic resins in different cases of partial edentations, with removable
partial dentures without metallic frame, or combining the metallic frame with thermoplastic
resin saddles, selected according to the requirements of the indications and manufacturing
technology- Fig. 2.
Fig. 2. Different combinations between thermoplastic resins. (a), (c) Without metal, (b) With
Manufacture of Different Types of Thermoplastic
The main characteristics of thermoplastic resins used are: they are monomer-free and
consequently non-toxic and non-allergenic, they are injected by using special devices, they
are biocompatible, they have enhanced esthetics and are comfortable at wearing.
The special injection devices we use are Polyapress (Bredent) and R-3C (Flexite) injectors-
Fig. 3. (a) The Polyapress injection-molding device (Bredent), (b) The R-3C injector (Flexite)
3. Manufacture technology for acetal-resin dentures
The acetal resin has optimal physical and chemical properties and it is indicated in making
frames and clasps for removable partial dentures, being available in tooth colour and in pink.
The denture acetal resin framework was combined with the use of acrylic resins at saddle
level (Fig. 2). As a particularity of the manuf